LMucko/crystallography-open-database huggingface dataset:
Considerable Improvement of Long-Persistent Luminescence in Germanium and Tin Substituted ZnGa2O4
Allix, Mathieu; Chenu, Sébastien; Véron, Emmanuel; Poumeyrol, Thomas; Kouadri-Boudjelthia, El Amin; Alahraché, Salaheddine; Porcher, Florence; Massiot, Dominique; Fayon, Franck; Chemistry of Materials 25 (2013) 1600–; doi:10.1021/cm304101n

data_4001768
_publ_section_title
;
 Considerable Improvement of Long-Persistent Luminescence in Germanium and
 Tin Substituted ZnGa2O4
;
_journal_issue                   9
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1600
_journal_paper_doi               10.1021/cm304101n
_journal_volume                  25
_journal_year                    2013
_chemical_formula_sum            'Ga1.8 Ge0.1 O4 Zn1.1'
_chemical_formula_weight         268.7
_chemical_name_systematic        ' ?'
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.33665(5)
_cell_length_b                   8.33665(5)
_cell_length_c                   8.33665(5)
_cell_measurement_temperature    293
_cell_volume                     579.395(6)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     1.2255
_exptl_absorpt_coefficient_mu    0.006
_exptl_crystal_density_diffrn    6.158
_exptl_crystal_F_000             992
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        121.000
_pd_meas_2theta_range_min        4.500
_pd_meas_number_of_points        2331
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        121
_pd_proc_2theta_range_min        4.5
_pd_proc_ls_background_function  '9 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.0297
_pd_proc_ls_prof_wR_expected     0.0127
_pd_proc_ls_prof_wR_factor       0.0384
_refine_ls_goodness_of_fit_all   3.02
_refine_ls_number_constraints    0
_refine_ls_number_parameters     23
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0149
_refine_ls_R_factor_gt           0.0149
_refine_ls_shift/su_max          0.0141
_refine_ls_shift/su_mean         0.0022
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.0246
_refine_ls_wR_factor_gt          0.0245
_cod_data_source_file            cm304101n_si_002.cif
_cod_data_source_block           I
_cod_original_sg_symbol_Hall     '-F 4abvw;2abvw;3'
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               4001768
Considerable Improvement of Long-Persistent Luminescence in Germanium and Tin Substituted ZnGa2O4
Allix, Mathieu; Chenu, Sébastien; Véron, Emmanuel; Poumeyrol, Thomas; Kouadri-Boudjelthia, El Amin; Alahraché, Salaheddine; Porcher, Florence; Massiot, Dominique; Fayon, Franck; Chemistry of Materials 25 (2013) 1600–; doi:10.1021/cm304101n

data_4001769
_publ_section_title
;
 Considerable Improvement of Long-Persistent Luminescence in Germanium and
 Tin Substituted ZnGa2O4
;
_journal_issue                   9
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1600
_journal_paper_doi               10.1021/cm304101n
_journal_volume                  25
_journal_year                    2013
_chemical_formula_sum            'Ga1.5 Ge0.25 O4 Zn1.25'
_chemical_formula_weight         268.4
_chemical_name_systematic        ' ?'
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.34115(4)
_cell_length_b                   8.34115(4)
_cell_length_c                   8.34115(4)
_cell_measurement_temperature    293
_cell_volume                     580.334(5)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     1.2252
_exptl_absorpt_coefficient_mu    0.006
_exptl_crystal_density_diffrn    6.143
_exptl_crystal_F_000             992
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        121.050
_pd_meas_2theta_range_min        4.500
_pd_meas_number_of_points        2332
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        121.05
_pd_proc_2theta_range_min        4.5
_pd_proc_ls_background_function  '9 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.0244
_pd_proc_ls_prof_wR_expected     0.0133
_pd_proc_ls_prof_wR_factor       0.0310
_refine_ls_goodness_of_fit_all   2.33
_refine_ls_number_constraints    0
_refine_ls_number_parameters     24
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0101
_refine_ls_R_factor_gt           0.0101
_refine_ls_shift/su_max          0.0742
_refine_ls_shift/su_mean         0.0051
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.0189
_refine_ls_wR_factor_gt          0.0189
_cod_data_source_file            cm304101n_si_003.cif
_cod_data_source_block           I
_cod_original_sg_symbol_Hall     '-F 4abvw;2abvw;3'
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               4001769
Considerable Improvement of Long-Persistent Luminescence in Germanium and Tin Substituted ZnGa2O4
Allix, Mathieu; Chenu, Sébastien; Véron, Emmanuel; Poumeyrol, Thomas; Kouadri-Boudjelthia, El Amin; Alahraché, Salaheddine; Porcher, Florence; Massiot, Dominique; Fayon, Franck; Chemistry of Materials 25 (2013) 1600–; doi:10.1021/cm304101n

data_4001770
_publ_section_title
;
 Considerable Improvement of Long-Persistent Luminescence in Germanium and
 Tin Substituted ZnGa2O4
;
_journal_issue                   9
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1600
_journal_paper_doi               10.1021/cm304101n
_journal_volume                  25
_journal_year                    2013
_chemical_formula_sum            'Ga Ge0.5 O4 Zn1.5'
_chemical_formula_weight         268.1
_chemical_name_systematic        ' ?'
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.35049(6)
_cell_length_b                   8.35049(6)
_cell_length_c                   8.35049(6)
_cell_measurement_temperature    293
_cell_volume                     582.285(7)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     1.2252
_exptl_absorpt_coefficient_mu    0.005
_exptl_crystal_density_diffrn    6.114
_exptl_crystal_F_000             992
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        121.050
_pd_meas_2theta_range_min        4.500
_pd_meas_number_of_points        2332
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        121.05
_pd_proc_2theta_range_min        7.05
_pd_proc_ls_background_function  '9 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.0323
_pd_proc_ls_prof_wR_expected     0.0155
_pd_proc_ls_prof_wR_factor       0.0456
_refine_ls_goodness_of_fit_all   2.94
_refine_ls_number_constraints    0
_refine_ls_number_parameters     24
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0108
_refine_ls_R_factor_gt           0.0108
_refine_ls_shift/su_max          0.0452
_refine_ls_shift/su_mean         0.0052
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.0185
_refine_ls_wR_factor_gt          0.0185
_cod_data_source_file            cm304101n_si_004.cif
_cod_data_source_block           I
_cod_original_sg_symbol_Hall     '-F 4abvw;2abvw;3'
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_original_formula_sum        'Ga1 Ge0.5 O4 Zn1.5'
_cod_database_code               4001770
Structure, Atomistic Simulations, and Phase Transition of Stoichiometric Yeelimite
Cuesta, Ana; De la Torre, Angeles G.; Losilla, Enrique R.; Peterson, Vanessa K.; Rejmak, Pawel; Ayuela, Andrés; Frontera, Carlos; Aranda, Miguel A. G.; Chemistry of Materials 25 (2013) 1680–; doi:10.1021/cm400129z

data_4001772
_publ_section_title
;
 Structure, Atomistic Simulations, and Phase Transition of Stoichiometric
 Yeelimite
;
_journal_issue                   9
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1680
_journal_paper_doi               10.1021/cm400129z
_journal_volume                  25
_journal_year                    2013
_chemical_formula_sum            'Al6 Ca4 O16 S'
_chemical_formula_weight         610.26
_space_group_IT_number           27
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2 -2c'
_symmetry_space_group_name_H-M   'P c c 2'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   13.0357(7)
_cell_length_b                   13.0350(7)
_cell_length_c                   9.16771(19)
_cell_measurement_temperature    298
_cell_volume                     1557.78(12)
_pd_block_id                     2012-07-25T10:13|REFINED_SOFTKLEIN_OR_phase2|||
_pd_phase_name                   'ORTHORHOMBIC Klein salt'
_cod_data_source_file            cm400129z_si_002.cif
_cod_data_source_block           REFINED_SOFTKLEIN_OR_phase_2
_cod_depositor_comments
;
 Changed the '_cod_related_entry' data name to '_cod_related_entry_code'.

 Antanas Vaitkus,
 2020-04-18

The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.3.1 from 2005-06-27 (182
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.3.1 from 2005-06-27 (385 times).

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        1557.78(6)
_cod_database_code               4001772
Molecular Salts of Anesthetic Lidocaine with Dicarboxylic Acids: Solid-State Properties and a Combined Structural and Spectroscopic Study
Braga, Dario; Chelazzi, Laura; Grepioni, Fabrizia; Dichiarante, Elena; Chierotti, Michele R.; Gobetto, Roberto; Crystal Growth & Design 13 (2013) 2564–2572; doi:10.1021/cg400331h

data_4507885
_publ_section_title
;
 Molecular Salts of Anesthetic Lidocaine with Dicarboxylic Acids:
 Solid-State Properties and a Combined Structural and Spectroscopic Study
;
_journal_coden_ASTM              CGDEFU
_journal_issue                   6
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              2564
_journal_page_last               2572
_journal_paper_doi               10.1021/cg400331h
_journal_volume                  13
_journal_year                    2013
_chemical_formula_moiety         'C18 H28 N2 O5'
_chemical_formula_sum            'C18 H28 N2 O5'
_chemical_formula_weight         352.43
_space_group_IT_number           19
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      19
_symmetry_space_group_name_Hall  'P 2ac 2ab'
_symmetry_space_group_name_H-M   'P 21 21 21'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   10.4949(30)
_cell_length_b                   10.8924(28)
_cell_length_c                   16.581(4)
_cell_measurement_temperature    295
_cell_volume                     1895.5(9)
_computing_cell_refinement       GSAS
_computing_data_collection       'Highscore plus'
_computing_structure_refinement  GSAS
_computing_structure_solution    'EXPO2011 (Altomare, 2011)'
_diffrn_ambient_temperature      293
_diffrn_radiation_monochromator  'Ge filtered'
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54056
_exptl_absorpt_coefficient_mu    0.739
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    1.235
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             760.0
_pd_proc_2theta_range_max        70
_pd_proc_2theta_range_min        5
_pd_proc_info_excluded_regions   no
_pd_proc_ls_background_function  Chebyschev
_pd_proc_ls_pref_orient_corr
;
Spherical Harmonics
;
_cod_data_source_file            cg400331h_si_003.cif
_cod_data_source_block           LIDOSUA01_phase_1
_cod_original_cell_volume        1895.45
_cod_database_code               4507885
Ba2YFeO5.5: A Ferromagnetic Pyroelectric Phase Prepared by Topochemical Oxidation.
Luo, Kun; Johnson, Roger D.; Tran, Thao T.; Halasyamani, P. Shiv; Radaelli, Paolo G.; Hayward, Michael A.; Chemistry of Materials 25 (2013) 1800–; doi:10.1021/cm400364y

data_4001780
_publ_section_title
;
 Ba2YFeO5.5: A Ferromagnetic Pyroelectric Phase Prepared by Topochemical
 Oxidation.
;
_journal_issue                   9
_journal_name_full               'Chemistry of Materials'
_journal_page_first              1800
_journal_paper_doi               10.1021/cm400364y
_journal_volume                  25
_journal_year                    2013
_chemical_formula_sum            'Ba2 Fe O5.5 Y'
_chemical_formula_weight         507.40
_space_group_IT_number           26
_symmetry_Int_Tables_number      26
_symmetry_space_group_name_Hall  'P -2 -2b'
_symmetry_space_group_name_H-M   'P b 21 m'
_audit_creation_date             13-04-04
_audit_creation_method           'Created with Diamond v2.0'
_audit_update_record             13-04-04
_cell_angle_alpha                90.000
_cell_angle_beta                 90.000
_cell_angle_gamma                90.000
_cell_formula_units_Z            4
_cell_length_a                   12.1320(2)
_cell_length_b                   6.0606(1)
_cell_length_c                   8.0956(1)
_cell_volume                     595.247(16)
_cod_data_source_file            cm400364y_si_002.cif
_cod_data_source_block           XXXX
_cod_depositor_comments
;
  The _chemical_formula_sum value was taken from the paper. The Z
  value was calculated from the cell contents to match the summary
  formula provided in the paper. The formula weight was recalculated
  from the new summary formula using atomic weights from
  http://www.webelements.com/. Old values are available in the
  _cod_original_* data items.

  Saulius Gra\<zulis
  2013-07-15
;
_cod_original_cell_volume        595.2(0)
_cod_original_sg_symbol_Hall     P_-2_-2b
_cod_original_formula_sum        'Ba8 Y4 Fe4 O22'
_cod_original_formula_weight     2029.614
_cod_database_code               4001780
Inorganic structure types with revised space groups.I.
Cenzual, K.; Gelato, L.M.; Penzo, M.; Parthe, E.; Acta Crystallographica B 47 (1991) 433–439; doi:10.1107/s0108768191000903

data_2105478
_publ_section_title
;
 Inorganic structure types with revised space groups.I.
;
_journal_name_full               'Acta Crystallographica B'
_journal_page_first              433
_journal_page_last               439
_journal_paper_doi               10.1107/s0108768191000903
_journal_volume                  47
_journal_year                    1991
_chemical_formula_structural     GaSe
_chemical_formula_sum            'Ga Se'
_chemical_name_systematic        'epsilon Gallium Selenide'
_space_group_IT_number           187
_symmetry_Int_Tables_number      187
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                120.
_cell_formula_units_Z            4
_cell_length_a                   3.743
_cell_length_b                   3.743
_cell_length_c                   15.919
_cell_volume                     193.146
_cod_data_source_file            GaSe_epsilon_P_6m2_DC240.cif
_cod_data_source_block           chateigner240
_cod_original_cell_volume        193.15
_cod_original_formula_sum        'Ga1 Se1'
_cod_database_code               2105478
Hochdrucksynthese und Strukturverfeinerung von SrVO~3~, Sr~2~VO~4~ und Sr~3~V~2~O~7~
Range, K. J.; Rau, F.; Klement, U.; Zeitschrift für Naturforschung B 46 (1991) 1315–1318; doi:10.1515/znb-1991-1006

data_7210231
_publ_section_title
;
 Hochdrucksynthese und Strukturverfeinerung von SrVO~3~, Sr~2~VO~4~ und
 Sr~3~V~2~O~7~
;
_journal_issue                   10
_journal_name_full               'Zeitschrift f\"ur Naturforschung B'
_journal_page_first              1315
_journal_page_last               1318
_journal_paper_doi               10.1515/znb-1991-1006
_journal_volume                  46
_journal_year                    1991
_chemical_formula_structural     'Sr V O2.93'
_chemical_formula_sum            'O2.93 Sr V'
_chemical_name_systematic        'Strontium Vanadium Oxide'
_space_group_IT_number           221
_symmetry_Int_Tables_number      221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            1
_cell_length_a                   3.8408(3)
_cell_length_b                   3.8408(3)
_cell_length_c                   3.8408(3)
_cell_volume                     56.659(8)
_cod_data_source_file            SrVO3_Pm-3m_DC241.cif
_cod_data_source_block           chateigner
_cod_original_cell_volume        56.66
_cod_original_formula_sum        'V1 Sr1 O2.93'
_cod_database_code               7210231
Synthesis, crystal structure, stoichiometry and magnetic properties of (Ca1-x Srx) V O3
Garcia-Jaca, J.; Mesa, J.L.; Insausti, M.; Larramendi, J.I.R.; Arriortua, M.I.; Rojo, T.; Materials Research Bulletin 34 (1999) 289–301; doi:10.1016/S0025-5408(99)00002-1

data_1512117
_publ_section_title
;
 Synthesis, crystal structure, stoichiometry and magnetic properties of
 (Ca1-x Srx) V O3
;
_journal_issue                   2
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              289
_journal_page_last               301
_journal_paper_doi               10.1016/S0025-5408(99)00002-1
_journal_volume                  34
_journal_year                    1999
_chemical_formula_structural     SrVO3)
_chemical_formula_sum            'O3 Sr V'
_chemical_name_systematic        'Strontium Vanadium Oxide'
_space_group_IT_number           221
_symmetry_Int_Tables_number      221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            1
_cell_length_a                   3.8409(1)
_cell_length_b                   3.8409(1)
_cell_length_c                   3.8409(1)
_cell_volume                     56.663(3)
_cod_data_source_file            SrVO3_Pm-3m_DC242.cif
_cod_data_source_block           chateigner
_cod_original_cell_volume        56.66
_cod_original_formula_sum        'Sr1 V1 O3'
_cod_database_code               1512117
Structure, magnetic susceptibility and resistivity properties of SrVO~3~
Lan, Y. C.; Chen, X. L.; He, M.; Journal of Alloys and Compounds 354 (2003) 95–98; doi:10.1016/S0925-8388(02)01349-X

data_1512118
_publ_section_title
;
 Structure, magnetic susceptibility and resistivity properties of SrVO~3~
;
_journal_issue                   1-2
_journal_name_full               'Journal of Alloys and Compounds'
_journal_page_first              95
_journal_page_last               98
_journal_paper_doi               10.1016/S0925-8388(02)01349-X
_journal_volume                  354
_journal_year                    2003
_chemical_formula_structural     SrVO3
_chemical_formula_sum            'O3 Sr V'
_chemical_name_systematic        'Strontium Vanadium Oxide'
_space_group_IT_number           221
_symmetry_Int_Tables_number      221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8425(1)
_cell_length_b                   3.8425(1)
_cell_length_c                   3.8425(1)
_cell_volume                     56.734(3)
_cod_data_source_file            SrVO3_Pm-3m_DC243.cif
_cod_data_source_block           chateigner
_cod_original_cell_volume        56.73
_cod_original_formula_sum        'Sr1 V1 O3'
_cod_database_code               1512118
Preparation and structure of the compounds Sr V O3 and Sr2 V O4
Rey, M.J.; Dehaudt, P.; Joubert, J.C.; Lambert Andron, B.; Cyrot, M.; Cyrot-Lackmann, F.; Journal of Solid State Chemistry 86 (1990) 101–108; doi:10.1016/0022-4596(90)90119-I

data_1512119
_publ_section_title
;
 Preparation and structure of the compounds Sr V O3 and Sr2 V O4
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              101
_journal_page_last               108
_journal_paper_doi               10.1016/0022-4596(90)90119-I
_journal_volume                  86
_journal_year                    1990
_chemical_formula_structural     SrVO3
_chemical_formula_sum            'O3 Sr V'
_chemical_name_systematic        'Strontium Vanadium Oxide'
_space_group_IT_number           221
_symmetry_Int_Tables_number      221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            1
_cell_length_a                   3.840(9)
_cell_length_b                   3.840(9)
_cell_length_c                   3.840(9)
_cell_volume                     56.6(2)
_cod_data_source_file            SrVO3_Pm-3m_DC244.cif
_cod_data_source_block           chateigner
_cod_original_cell_volume        56.62
_cod_original_formula_sum        'Sr1 V1 O3'
_cod_database_code               1512119